[Integrated Circuits and Systems] Applications of Organic and Printed Electronics || High Efficiency OLEDs for Lighting Applications
Post on 12-Dec-2016
Embed Size (px)
Chapter 4High Efficiency OLEDs for LightingApplications
Completing the Solid State LightingPortfolio
Reinder Coehoorn, Volker van Elsbergenand Coen Verschuren
Abstract Organic Light-Emitting Diode (OLED) technology is developing as apromising option for large area lighting applications, with basic properties such asefficiency, color stability and lifetime which approach or even exceed those ofconventional lighting and inorganic LED technology and with various interestingadditional complementing features. In this Chapter, an introduction is given on thedevelopment of OLED technology for lighting applications. We discuss theworking principles of efficient white multilayer OLEDs, the factors which deter-mine the efficiency, several key elements of the fabrication technology includingencapsulation methods, and the state-of-the-art as realized in various institutes andcompanies.
Keywords OLED Lighting Charg-carrier mobility Efficiency Lifetime Fluorescence Phosphorescence Fabrication Encapsulation
Organic Light-Emitting Diodes (OLEDs) are thin-film solid state lighting devices,consisting of an organic semiconducting layer or layer stack which is sandwiched inbetween two electrode layers. When a voltage is applied across the organic layer,
R. Coehoorn (&) C. VerschurenPhilips Research Laboratories, High Tech Campus 4,5656 AE Eindhoven, The Netherlandse-mail: firstname.lastname@example.org
V. van ElsbergenPhilips Research Laboratories, Weisshausstrasse 2,D-52066 Aachen, Germany
E. Cantatore (ed.), Applications of Organic and Printed Electronics,Integrated Circuits and Systems, DOI: 10.1007/978-1-4614-3160-2_4, Springer Science+Business Media New York 2013
the injection of electrons and holes from the cathode and anode, respectively, givesrise to an electrical current. The subsequent radiative recombination of the injectedelectrons and holes in the organic layer leads to light emission. Emission in aspecific organic compound is usually confined to a relatively broad wavelengthrange, typically 70100 nm wide. Using a combination of three organic layers, withpredominant blue, green and red emission, white light emission can be obtained.Figure 4.1 shows warm and cold white OLEDs, and a comparison with conven-tional light sources.
In Fig. 4.2 a more quantitative comparison of OLEDs with other light sources ismade. Recent advances have led to values of the luminous efficacy of more than60 lm W-1 at present, using rough foils for improving the light-outcouplingefficiency, or to values well above 60 lm W-1 using more special methods forimproving the light-outcoupling efficiency, as discussed in Sect. 4.2. The highestpossible luminous efficacy for a high quality white light source is approximately300 lm W-1. The system efficiency given in Fig. 4.2 is taken to be the luminousefficacy expressed as a percentage of this maximum efficacy. Another quantityof interest is the lamp efficiency. OLEDs are by nature large-area light sources,which operate typically at 1000 cd m-2 for decorative applications, and at30005000 cd m-2 for general lighting applications. No special luminaire for lightdiffusion and for cooling is then necessary, so that there is no related reduction ofthe lamp efficiency. Natural cooling at the ambient air is sufficient. White OLEDlifetimes can exceed more than 10,000 h, as discussed in more detail in Sect. 4.4.
The relatively broad emission spectra from organic materials make it possiblethat white OLEDs containing three emitting layers can have a very high ColorRendering Index (CRI), up to 90 or more. The CRI expresses the degree to whichemission colors of all wavelengths in the visible range are present, which deter-mines the naturalness and vividness of the colors reflected from illuminatedobjects, i.e. the pleasantness of the light source. It is a number in between 0(bad) and 100 (excellent).
Whereas to-date standard OLEDs are produced by deposition on a thin rigidglass substrate, the small thickness of the active layers and the electrode layers(only a few hundreds of nanometres in total) makes it possible to produce OLEDs
Fig. 4.1 OLEDs (warm andcold white) as compared toconventional light sources(compact fluorescent (CFL),incandescent and fluorescent(TL) lamps)
84 R. Coehoorn et al.
which are flexible and even bendable by deposition on e.g. a polymer foil.Figure 4.3 shows an example of such an OLED. This is expected to open upentirely new areas of applications. Additional demonstrated features of whiteOLEDs are the operation at safe low voltages (close to the thermodynamic limit ofapproximately 3 V), easy dimmability, the possibility to tune the emission color,and the possibility to create OLEDs which are transparent in the off-state andemissive to both sides in the on-state (using two conductive transparent electrodelayers). At present, color-neutral transparencies of approximately 75 % have beendemonstrated.
In view of these prospects, various companies based in the Europe, Asia and theUS are developing OLEDs for white lighting applications. A review has recentlybeen presented by Loebl et al. . Philips was, in 2008, the first company tocommercialize OLED lighting products. Under the name LUMIBLADETM
(www.the-new-art-of-light.com/), a catalogue collection of OLEDs with differentshapes, sizes and colors became available (Fig. 4.4).
Fig. 4.2 Comparison of various technologies for white lighting applications. For LED andOLED technology, which are still under development, the numbers in between parentheses givethe estimated technologically achieveable maximum. For both technologies, the luminousefficacy at brightness levels well below the reference value of 1000 cd m-2 can be significantlylarger than the values given
Fig. 4.3 Flexible whiteOLED (Source http://www.holstcentre.com/NewsPress).Photograph reproduced withpermission of the HolstCentre (Eindhoven, TheNetherlands)
4 High Efficiency OLEDs for Lighting Applications 85
In Sect. 4.2, we discuss the structure and functioning of white OLEDs forlighting applications, and in Sect. 4.3 we discuss the fabrication technologies used.Encapsulation technologies are discussed in Sect. 4.4. In Sect. 4.5 the prospects forlighting applications are discussed. An overview of excellent reviews of OLEDtechnology is given in Refs. .
4.2 Functioning of OLEDs
OLEDs are based on organic materials within which the bond between the carbonatoms is alternatingly single and double (p-conjugated materials), so that they canfunction as (intrinsic) semiconductors which conduct when charge is injected fromthe electrodes. The standard text which describes the physics of electronic pro-cesses in organic materials is the book of Pope and Svenberg . Figure 4.5 showsvarious examples of conjugated organic materials used in OLEDs. As demon-strated first by Tang van VanSlyke , it is possible to fabricate OLEDs on thebasis of one or more evaporation deposited layers of small molecules, such asaluminium tris(8-hydroxyquinoline) (Alq3, Fig. 4.5a). In 1990, Friend andco-workers showed that it is also possible to fabricate OLEDs using spin-coatingdeposited polymers, such as poly-phenylene-vinylene (PPV). The structure of atypical so-called bottom emitting OLEDs is as follows:
substrate (glass or a transparent polymer), transparent anode layer (e.g. *150 nm indium-tin-oxide, ITO), the active organic semiconductor layer stack (*80120 nm), cathode (e.g. an aluminium layer of typically 100 nm with a few nanometers of
LiF, Ba or Ca layer at the interface in order to improve the electron injection),
Fig. 4.4 OLEDs fromPhilips Lumiblade,www.the-new-art-of-light.com/
86 R. Coehoorn et al.
a metal, a glass lid or a thin film encapsulating layer structure which protects thecathode from the air and water in the ambient atmosphere.
The active organic semiconductor layer stack can, in principle, consist of asingle organic layer containing a mixture of molecules emitting at different
(a) (b) (c) (d)
Fig. 4.5 Examples of organic materials used in OLEDs. a aluminium-tris-(8-hydroxy-quinolin)(Alq3, EML and ETL, see Fig. 4.6). b iridium(III) bis(2-(20-benzothienyl) pyridinato-M,C30)(acetylacetonate) (btp2Ir(acac), red phosphorescent dopant). c fac-tris(2-phenylpyridine)iridium(Ir(ppy)3, green phosphorescent dopant). d bis(2-(4,6-difluorophenyl)pyridyl-N,C20)iridium(acetylacetonate) (FIrpic, blue phosphorescent dopant)
Fig. 4.6 a Schematic structure of a multilayer small-molecule bottom emitting OLED.b Schematic energy diagram showing the functioning of the OLED. It contains hole and electroninjection layers (HIL, EIL), hole and electron transport layers (HTL, ETL), electron and holeblocking layers (EBL, HBL), and an emissive layer (EML) containing red, green and blue emittingdye molecules (with LUMO and HOMO energies indicated by dashed lines). The figure shows theflat band situation (neglecting the effects of space charge in the layers on the actual positiondependence of the HOMO and LUMO levels). EF is the Fermi energy, and V is the applied voltage
4 High Efficiency OLEDs for Lighting Applications 87
wavelengths. However, in the most efficient white OLEDs which are presentlydeveloped for general lighting applications, the active organic layer consists ofmany sublayers, each fulfilling a specific function. A typical example is given inFig. 4.6a.
Figure 4.6b gives the energy landscape in the OLED at a voltage equal to thebuilt-in voltage, Vbi, which is the effective work function difference between theanode and the cathode. The figure shows, firstly, the injection of electrons andholes from the Fermi level energy (EF) in the cathode and anode, respectively, intothe lowest unoccupied molecular orbital (LUMO) states and the highest occupiedmolecular orbital (HOMO) states of the organic semiconductors used (curvedarrows). The HOMO and LUMO states are separated by an energy gap (whitezone). Efficient electron and hole injection can only take place from electrodelayers with a low and a high effective work function, respectively. For simplicity,the figure neglects the effects of the presence of the injected space charge in theOLED, which is in actual devices quite important, causing band bending. Forvoltages 0 \ V \ Vbi, only a very small current can flow, due to charge carrierdiffusion. In a properly designed OLED, with small injection barriers, the OLEDturns on at V & Vbi. The Coulomb attraction between the injected electrons andholes leads to the formation of bound electronhole pairs (excitons), which canrecombine radiatively to form a photon, which gives rise to light emission.
The zone within which the emission takes place is confined to an emissive layer(EML) in the center, in order to maximize the efficiency of light-outcoupling out ofthe microcavity. This efficiency is relatively small for emission close to theelectrodes, due to fast irreversible energy transfer to the electrodes. For this pur-pose, use is made of a combination of electron and hole transport layers (ETL andHTL, respectively) and electron and hole blocking layers (EBL and HBL,respectively) at either side of the EML. The emissive layer (EML) consists usuallyof at least three sublayers, giving rise to red, green and blue emission, so thatoverall white emission at a color coordinate very close to the black body curve isobtained with a correlated color temperature which depends on the requiredapplication (varying from 2700 K, warm white, to above 4000 K, cold white)and with a high CRI. The electron and hole transport layers separate the EML fromthe electrodes, and should have a large electron and hole mobility, respectively, inorder to assure that the voltage drop is confined mainly to the EML. Efficientinjection into the transport layers can be obtained by making use of n-doped andp-doped electron and hole injection layers (EIL and HIL) at the anode and cathodeinterfaces, respectively . The conductivity of these layers is very high,resulting in a negligible voltage drop.
The efficiency of the emission within each sublayer within the EML depends, inthe first place, on the quantummechanical nature of the excitons formed. Inorganic materials based on only light atoms, such as carbon, oxygen, nitrogen andhydrogen, one may strictly distinguish singlet excitons (total spin quantum numberS = 0) and triplet excitons (S = 1). Radiative decay of singlet excitons to the(S = 0) ground state, called fluorescence, is a quantum-mechanically allowedprocess and occurs usually within 110 ns. In contrast, radiative decay of triplet
88 R. Coehoorn et al.
excitons to the ground state, called phosphorescence, is a quantum-mechanicallyforbidden process. From quantum statistics, it is expected that exciton formationbetween electrons and holes with uncorrelated spins leads to singlet and tripletexcitons in a ratio of 1:3. In OLEDs based on fluorescent emitters, the emissionefficiency is therefore severely limited by the small singlet fraction, gS = 0.25. Influorescent emitters, the triplet exciton lifetime is very long, sometimes more than1 ms. Almost all triplets decay non-radiatively after diffusion to quenching sites.Experimental studies suggest that gS is indeed close to 0.25 for small-moleculematerials based on only light elements, but it has been argued that it is significantlylarger for some polymers [12, 13].
The OLED efficiency can be increased drastically by making use of organicmaterials in which heavy metal atoms such as Ir or Pt are present, in which spinorbit interaction gives rise to a relatively strong admixture of singlet character intootherwise predominantly triplet states . In such phosphorescent emitters ortriplet-emitters, such as the Ir-dye molecules shown in Fig. 4.5bd, the radiativelifetime is decreased to typically 1 ls, and efficient emission from excitons withpredominant singlet and triplet character is obtained. The phosphorescent mole-cules are often present as red, green and blue dopants in a host material with a highenergy gap. The corresponding HOMO and LUMO energy levels are indicated asdashed lines in Fig. 4.6b.
For fluorescent OLEDs, the external quantum efficiency (EQE, gEQE, defined asthe total number of emitted photons as measured in an integrating sphere spec-trometer  per electron passing the device) is determined by four factors:
gEQE gef gSgradglo: 4:1Here, gef is the exciton formation efficiency, i.e. the fraction of the injected carrierswhich actually form an exciton, gS is the singlet fraction discussed above, grad is thesinglet exciton radiative decay probability and glo is the light-outcoupling effi-ciency. For phosphorescent OLEDs, within which all excitons can emit,gEQE gefgradglo. In multilayer OLEDs containing electron and hole blockinglayers, gef is very close to 1. The radiative decay probability, which is limited by thediffusion of excitons to quenching sites, can be maximized by appropriate chemicalsynthesis and...